Md Tusher Mollah Raphaël 사령관 Marcin P. Serdeczny David B. Pedersen Jon Spangenberg덴마크 공과 대학 기계 공학과, Kgs. 덴마크 링비
2020년 12월 22일 접수, 2021년 5월 1일 수정, 2021년 7월 15일 수락, 2021년 7월 21일 온라인 사용 가능, 기록 버전 2021년 8월 17일 .
이 문서는 재료 압출 적층 제조 에서 여러 레이어를 인쇄하는 동안 증착 흐름의 전산 유체 역학 시뮬레이션 을 제공합니다 . 개발된 모델은 증착된 레이어의 형태를 예측하고 점소성 재료 를 인쇄하는 동안 레이어 변형을 캡처합니다 . 물리학은 일반화된 뉴턴 유체 로 공식화된 Bingham 구성 모델의 연속성 및 운동량 방정식에 의해 제어됩니다. . 증착된 층의 단면 모양이 예측되고 재료의 다양한 구성 매개변수에 대해 층의 변형이 연구됩니다. 층의 변형은 인쇄물의 정수압과 압출시 압출압력으로 인한 것임을 알 수 있다. 시뮬레이션에 따르면 항복 응력이 높을수록 변형이 적은 인쇄물이 생성되는 반면 플라스틱 점도 가 높을수록 증착된 레이어에서변형이 커 집니다 . 또한, 인쇄 속도, 압출 속도 의 영향, 층 높이 및 인쇄된 층의 변형에 대한 노즐 직경을 조사합니다. 마지막으로, 이 모델은 후속 인쇄된 레이어의 정수압 및 압출 압력을 지원하기 위해 증착 후 점소성 재료가 요구하는 항복 응력의 필요한 증가에 대한 보수적인 추정치를 제공합니다.
This paper presents computational fluid dynamics simulations of the deposition flow during printing of multiple layers in material extrusion additive manufacturing. The developed model predicts the morphology of the deposited layers and captures the layer deformations during the printing of viscoplastic materials. The physics is governed by the continuity and momentum equations with the Bingham constitutive model, formulated as a generalized Newtonian fluid. The cross-sectional shapes of the deposited layers are predicted, and the deformation of layers is studied for different constitutive parameters of the material. It is shown that the deformation of layers is due to the hydrostatic pressure of the printed material, as well as the extrusion pressure during the extrusion. The simulations show that a higher yield stress results in prints with less deformations, while a higher plastic viscosity leads to larger deformations in the deposited layers. Moreover, the influence of the printing speed, extrusion speed, layer height, and nozzle diameter on the deformation of the printed layers is investigated. Finally, the model provides a conservative estimate of the required increase in yield stress that a viscoplastic material demands after deposition in order to support the hydrostatic and extrusion pressure of the subsequently printed layers.
점성 플라스틱 재료, 재료 압출 적층 제조(MEX-AM), 다층 증착, 전산유체역학(CFD), 변형 제어
Viscoplastic Materials, Material Extrusion Additive Manufacturing (MEX-AM), Multiple-Layers Deposition, Computational Fluid Dynamics (CFD), Deformation Control
Three-dimensional printing of viscoplastic materials has grown in popularity over the recent years, due to the success of Material Extrusion Additive Manufacturing (MEX-AM) . Viscoplastic materials, such as ceramic pastes [2,3], hydrogels , thermosets , and concrete , behave like solids when the applied load is below their yield stress, and like a fluid when the applied load exceeds their yield stress . Viscoplastic materials are typically used in MEX-AM techniques such as Robocasting , and 3D concrete printing [9,10]. The differences between these technologies lie in the processing of the material before the extrusion and in the printing scale (from microscale to big area additive manufacturing). In these extrusion-based technologies, the structure is fabricated in a layer-by-layer approach onto a solid surface/support [11, 12]. During the process, the material is typically deposited on top of the previously printed layers that may be already solidified (wet-on-dry printing) or still deformable (wet-on-wet printing) . In wet-on-wet printing, control over the deformation of layers is important for the stability and geometrical accuracy of the prints. If the material is too liquid after the deposition, it cannot support the pressure of the subsequently deposited layers. On the other hand, the material flowability is a necessity during extrusion through the nozzle. Several experimental studies have been performed to analyze the physics of the extrusion and deposition of viscoplastic materials, as reviewed in Refs. [13–16]. The experimental measurements can be supplemented with Computational Fluid Dynamics (CFD) simulations to gain a more complete picture of MEX-AM. A review of the CFD studies within the material processing and deposition in 3D concrete printing was presented by Roussel et al. . Wolfs et al.  predicted numerically the failure-deformation of a cylindrical structure due to the self-weight by calculating the stiffness and strength of the individual layers. It was found that the deformations can take place in all layers, however the most critical deformation occurs in the bottom layer. Comminal et al. [19,20] presented three-dimensional simulations of the material deposition in MEX-AM, where the fluid was approximated as Newtonian. Subsequently, the model was experimentally validated in Ref.  for polymer-based MEX-AM, and extended to simulate the deposition of multiple layers in Ref. , where the previously printed material was assumed solid. Xia et al.  simulated the influence of the viscoelastic effects on the shape of deposited layers in MEX-AM. A numerical model for simulating the deposition of a viscoplastic material was recently presented and experimentally validated in Refs.  and . These studies focused on predicting the cross-sectional shape of a single printed layer for different processing conditions (relative printing speed, and layer height). Despite these research efforts, a limited number of studies have focused on investigating the material deformations in wet-on-wet printing when multiple layers are deposited on top of each other. This paper presents CFD simulations of the extrusion-deposition flow of a viscoplastic material for several subsequent layers (viz. three- and five-layers). The material is continuously printed one layer over another on a fixed solid surface. The rheology of the viscoplastic material is approximated by the Bingham constitutive equation that is formulated using the Generalized Newtonian Fluid (GNF) model. The CFD model is used to predict the cross-sectional shapes of the layers and their deformations while printing the next layers on top. Moreover, the simulations are used to quantify the extrusion pressure applied by the deposited material on the substrate, and the previously printed layers. Numerically, it is investigated how the process parameters (i.e., the extrusion speed, printing speed, nozzle diameter, and layer height) and the material rheology affect the deformations of the deposited layers. Section 2 describes the methodology of the study. Section 3 presents and discusses the results. The study is summarized and concluded in Section 4.
 R.A. Buswell, W.R. Leal De Silva, S.Z. Jones, J. Dirrenberger, 3D printing using
concrete extrusion: a roadmap for research, Cem. Concr. Res. 112 (2018) 37–49.
 Z. Chen, Z. Li, J. Li, C. Liu, C. Lao, Y. Fu, C. Liu, Y. Li, P. Wang, Y. He, 3D printing of
ceramics: a review, J. Eur. Ceram. Soc. 39 (4) (2019) 661–687.
 A. Bellini, L. Shor, S.I. Guceri, New developments in fused deposition modeling of
ceramics, Rapid Prototyp. J. 11 (4) (2005) 214–220.
 S. Aktas, D.M. Kalyon, B.M. Marín-Santib´
anez, ˜ J. P´erez-Gonzalez, ´ Shear viscosity
and wall slip behavior of a viscoplastic hydrogel, J. Rheol. 58 (2) (2014) 513–535.
 J. Lindahl, A. Hassen, S. Romberg, B. Hedger, P. Hedger Jr., M. Walch, T. Deluca,
W. Morrison, P. Kim, A. Roschli, D. Nuttall, Large-scale Additive Manufacturing
with Reactive Polymers, Oak Ridge National Lab.(ORNL), Oak Ridge, TN (United
 V.N. Nerella, V. Mechtcherine, Studying the printability of fresh concrete for
formwork-free Concrete onsite 3D Printing Technology (CONPrint3D), 3D Concr.
Print. Technol. (2019) 333–347.
 C. Tiu, J. Guo, P.H.T. Uhlherr, Yielding behaviour of viscoplastic materials, J. Ind.
Eng. Chem. 12 (5) (2006) 653–662.
 B. Dietemann, F. Bosna, M. Lorenz, N. Travitzky, H. Kruggel-Emden, T. Kraft,
C. Bierwisch, Modeling robocasting with smoothed particle hydrodynamics:
printing gapspanning filaments, Addit. Manuf. 36 (2020), 101488.
 B. Khoshnevis, R. Russell, H. Kwon, S. Bukkapatnam, Contour crafting – a layered
fabrication, Spec. Issue IEEE Robot. Autom. Mag. 8 (3) (2001) 33–42.
 D. Asprone, F. Auricchio, C. Menna, V. Mercuri, 3D printing of reinforced concrete
elements: technology and design approach, Constr. Build. Mater. 165 (2018)
 J. Jiang, Y. Ma, Path planning strategies to optimize accuracy, quality, build time
and material use in additive manufacturing: a review, Micromachines 11 (7)
 J. Jiang, A novel fabrication strategy for additive manufacturing processes,
J. Clean. Prod. 272 (2020), 122916.
 F. Bos, R. Wolfs, Z. Ahmed, T. Salet, Additive manufacturing of concrete in
construction: potentials and challenges, Virtual Phys. Prototyp. 11 (3) (2016)
 P. Wu, J. Wang, X. Wang, A critical review of the use of 3-D printing in the
construction industry, Autom. Constr. 68 (2016) 21–31.
 T.D. Ngo, A. Kashani, G. Imbalzano, K.T. Nguyen, D. Hui, Additive manufacturing
(3D printing): a review of materials, methods, applications and challenges,
Compos. Part B: Eng. 143 (2018) 172–196.
 M. Valente, A. Sibai, M. Sambucci, Extrusion-based additive manufacturing of
concrete products: revolutionizing and remodeling the construction industry,
J. Compos. Sci. 3 (3) (2019) 88.
 N. Roussel, J. Spangenberg, J. Wallevik, R. Wolfs, Numerical simulations of
concrete processing: from standard formative casting to additive manufacturing,
Cem. Concr. Res. 135 (2020), 106075.
 R.J.M. Wolfs, F.P. Bos, T.A.M. Salet, Early age mechanical behaviour of 3D printed
concrete: numerical modelling and experimental testing, Cem. Concr. Res. 106
 R. Comminal, M.P. Serdeczny, D.B. Pedersen, J. Spangenberg, Numerical modeling
of the strand deposition flow in extrusion-based additive manufacturing, Addit.
Manuf. 20 (2018) 68–76.
 R. Comminal, M.P. Serdeczny, D.B. Pedersen, J. Spangenberg, Numerical modeling
of the material deposition and contouring precision in fused deposition modeling,
in Proceedings of the 29th Annual International Solid Freeform Fabrication
Symposium, Austin, TX, USA, 2018, pp. 1855–1864.
 M.P. Serdeczny, R. Comminal, D.B. Pedersen, J. Spangenberg, Experimental
validation of a numerical model for the strand shape in material extrusion additive
manufacturing, Addit. Manuf. 24 (2018) 145–153.
 M.P. Serdeczny, R. Comminal, D.B. Pedersen, J. Spangenberg, Numerical
simulations of the mesostructure formation in material extrusion additive
manufacturing, Addit. Manuf. 28 (2019) 419–429.
 H. Xia, J. Lu, G. Tryggvason, A numerical study of the effect of viscoelastic stresses
in fused filament fabrication, Comput. Methods Appl. Mech. Eng. 346 (2019)
 R. Comminal, W.R.L. da Silva, T.J. Andersen, H. Stang, J. Spangenberg, Influence
of processing parameters on the layer geometry in 3D concrete printing:
experiments and modelling, in: Proceedings of the Second RILEM International
Conference on Concrete and Digital Fabrication, vol. 28, 2020, pp. 852–862.
 R. Comminal, W.R.L. da Silva, T.J. Andersen, H. Stang, J. Spangenberg, Modelling
of 3D concrete printing based on computational fluid dynamics, Cem. Concr. Res.
38 (2020), 106256.
 E.C. Bingham, An investigation of the laws of plastic flow, US Bur. Stand. Bull. 13
 N. Casson, A flow equation for pigment-oil suspensions of the printing ink type,
Rheol. Disperse Syst. (1959) 84–104.
 W.H. Herschel, R. Bulkley, Konsistenzmessungen von Gummi-Benzollosungen, ¨
Kolloid Z. 39 (1926) 291–300.
 “FLOW-3D | We solve The World’s Toughest CFD Problems,” FLOW SCIENCE.
〈https://www.flow3d.com/〉. (Accessed 27 June 2020).
 S. Jacobsen, R. Cepuritis, Y. Peng, M.R. Geiker, J. Spangenberg, Visualizing and
simulating flow conditions in concrete form filling using pigments, Constr. Build.
Mater. 49 (2013) 328–342.
 E.J. O’Donovan, R.I. Tanner, Numerical study of the Bingham squeeze film
problem, J. Non-Newton. Fluid Mech. 15 (1) (1984) 75–83.
 C.W. Hirt, B.D. Nichols, Volume of fluid (VOF) method for the dynamics of free
boundaries, J. Comput. Phys. 39 (1) (1981) 201–225.
 R. Comminal, J. Spangenberg, J.H. Hattel, Cellwise conservative unsplit advection
for the volume of fluid method, J. Comput. Phys. 283 (2015) 582–608.
 A. Negar, S. Nazarian, N.A. Meisel, J.P. Duarte, Experimental prediction of material
deformation in large-scale additive manufacturing of concrete, Addit. Manuf. 37